Electro Optical Characterisation of Short Wavelength Semiconductor ...
Chapter 5 Summary and Outlook Great things are not done by impulse, but by a series of small things brought together. Vincent van Gogh The main focus of this thesis has been opto-electrical characterisation of the laser diodes made in the semiconductor epitaxy group in Bremen. These are subcategorised in two main streams; the II-VI group and the III-V group based semiconductor lasers. The growth and the processing steps were all done internally. Therefore, it was a great situation to get familiar to the wide world of epitaxy and the proceeding device processing technology. Structural characterisation, even not belonging to the narrow issue of this thesis in comparison to the whole job being done in the group, is vital. Only through the feedbacks hereby and by the opto-electrical characterisation is reaching an optimal laser diode possible. And like any other characterisation theses the optimisation remarks are the last words said. The crystal quality of the ZnSe laser diodes pretty fine (putting aside the fact that the ZnSe based lasers have generally low lifetimes). As the measurements in the thesis show the most efforts should be done by the processing technology to make devices with narrow and deep ridges. This helps the reducing of the threshold current density and consequently less heat. The lifetime of the devices are then influenced positively. As a remark, since dealing with the 2µm structures is no easy task and on the other hand the optimum of the measured devices was by the 6µm, new structures can be processed in all ridge widths possible between 6µm and 2µm to obtain the optimal results for the reachable accuracy. Another point to mention in this connection is that wet etching could often make life much easier. This method, if controlled, could lead to faster and more uniform processing of devices. Some attempts during the technology steps of preparing the samples of this thesis showed the difficulties. But it’s worth continuing. No ZnSe laser would even come to the idea to light with the impurities which are the case by the GaNs. This intractable feature possibly constitutes the attractiveness of GaN. On the other hand reaching a crystal with less impurities is a tough task. This is the long-term aim of the growers. Like in case of ZnSe reaching the 2µm ridge widths is desired but not easy at all. Improvements in technology steps could realise this wish, due to which and hand in hand with improving the crystal quality a long lifetime and a reasonable consumption is guaranteed. The idea of making the cladding layer thicker in order to reduce or even stop the substrate luminescence needs to be developed with having in mind that too thick layers lead to a 53
University of Bremen Technical Univ
Preface ing the characterisation me